research article development of hpdc advanced dies by casting research article development of hpdc...
Post on 20-Feb-2020
Embed Size (px)
Research Article Development of HPDC Advanced Dies by Casting with Reinforced Tool Steels
I. Vicario,1 J. K. Idoiaga,2 E. Arratibel,3 I. Erauskin,1
L. M. Plaza,1 I. Crespo,1 and P. Caballero1
1Tecnalia Research & Innovation, 20009 San Sebastián, Spain 2Industrias Lebario, 48213 Izurza, Spain 3Fundiciones Inyectadas Alavesas S.A., 01230 Nanclares de la Oca, Spain
Correspondence should be addressed to I. Vicario; email@example.com
Received 26 August 2014; Accepted 11 January 2015
Academic Editor: Jean-Yves Hascoet
Copyright © 2015 I. Vicario et al.This is an open access article distributed under the Creative CommonsAttribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.
High pressure die casting (HPDC) dies are nowadays manufactured with high quality forged steels. Cavities are made by electrical discharge machining (EDM) or by high speed milling. The average life of an aluminium HPDC die is about 125.000 injections. Refrigeration circuits have simple configurations, because they are produced by drilling the die with straight holes. They are limitations in the distances and diameters of holes. Sensors are placed where the geometry of the die permits an easy machining. In order to obtain complex figures, several rapid prototyping methods have been developed. However, there is a limitation in the life of the dies produced by this technique, from several parts to thousands. A new method to obtain semifinished high pressure die casting dies in a steel of higher mechanical properties and with the refrigeration circuits and sensors embedded into it is described in this paper. The method consists in producing a molten steel alloy with micro-nano-special ceramic particles inserted in it and casting the composite material in sand moulds of the desired geometry.The resultant solidified near-net shape die with the cooling tubes and sensors embedded into it. A use-life and a productivity about 50% and 10% higher are obtained.
In the last years HPDC cast parts have developed a quick development due to the high automation, the new die materials, and sensoring and construction methods and also by the advanced control and foundry systems.
HPDC are generally made in H11 or H13 steel alloys by high speed machining combined with electrical discharge machining (EDM). Dies are expensive, due to the expensive tooling and the high energy and man power demanded in these operations.
Rapid prototyping processes are coming more and more employed in HPDCmoulds, but they are employed normally for first series, because the properties obtained with those parts produced by this technology cannot obtain the same life time thanwith standard fabricated dies. According to bibliog- raphy [1–3], there are different direct metal part production methods to made dies by rapid prototyping process. Between
them, the direct metal laser sintering (DMLS) and selective laser sintering (SLS) offers the possibility to adapt the cooling channels to the contour of a cavity without limitations in the form, optimizing die temperature control and increasing the die life. Cycle time reductions can be also obtained by optimizing the cooling circuits, and quality is increased by the nonquality parts reject reduction due to a better thermal stability of the die. However, there are several constraints to employ some alloys as the H11, and the metallurgical quality of produced parts is not as good as forged pieces used for dies.
There are also several indirect metal part production methods . These processes have been employed for insert fabrication, but their applications are very limited.
The steel sand casting technique has been also appointed as a possible way to construct cavities and dies . There is a reduction in the fabrication time, is necessary less raw material andmachining operations are reduced.However, the application of those products is limited for first series and for
Hindawi Publishing Corporation International Journal of Manufacturing Engineering Volume 2015, Article ID 287986, 10 pages http://dx.doi.org/10.1155/2015/287986
2 International Journal of Manufacturing Engineering
Table 1: Temper temperatures and materials.
460∘C 580∘C 600∘C Base alloy e e Reinforced alloy e e e
the supporting parts of the dies, due to the limited lifetime of the dies and the necessity of machining the refrigerating circuits.
One of the main mechanisms that define the total life of a die is the thermal fatigue cracking [6, 7]. In order to increase die life, new hot work tool steels with improved properties for HPDC applications are being continuously developed [8, 9].
Between them, the metal matrix composites have the potential to increase the thermal fatigue property [10, 11].
This work deals mainly with the development of a foundry process to produce HPDC dies with customised internal refrigeration and high resistance new steel. The objective is to obtain an economical process to produce advanced HPDC dies.
2. Design of Experiments
Thebasematerial for the tests has been chosen from themost employed steels used by HPDC die makers. The alloy 1.2344 (H13) was finally elected.
Based on the previous experience, in order to reinforce the base material, a Fe(TiMo)C master-alloy produced by self-propagating high temperature synthesis (SHS) has been chosen to be added to liquid steel.
To compare the new developed material properties in function of different tempering temperatures, some test bars were casted, heat-treated, and machined. An industrial induction furnace was used to prepare 300 kg of molten steel from selected scraps.When the scraps were melted at 1650∘C, the steel was dedrossed and a 7.5% in weight of Fe(TiMo)C master alloy was added until a good dissolutionwas obtained. Test bars were poured in sand moulds at 1.550∘C. After the solidification, parts were demoulded and separated from runners and overflows. Test wars were quenched at 890∘C for 2 hours and tempered at temperatures between 460 and 600∘C for 2 hours. After sand blasting, parts were machined in a high speed milling machine.
For the mechanical characterization, standard EN- 10002.1, EN-10045.1, and EN-10003.1 bars were machined to test tensile, resilience, and hardness properties, respectively. Wearing properties were also checked by pin on disk test. Thermal test bars have a dimension of 150 × 50 × 50mm with internal channels of 20mmofwidth, 5mmof depth, and 110mm length (see Figure 1(a)). The test bars were essayed in a test machine during 100.000 cycles and with a variation of temperature from 600 to 250∘C every 30 s, by induction heating and followed then by water and air spraying.
The two cast materials were quenched at 890∘C and tempered at different temperatures (see Table 1) in order to determinate the differences between materials and the optimum temper temperature for HPDC die applications.
Table 2: Tube sizes, fillers, and positions.
Ref. Outside diameter (mm)
Inside diameter (mm)
Filler Tube position
1 10 7 Gas Vertical 2 18 9 Sand Vertical 3 17 11 Sand Vertical 4 8 5.4 — Horizontal 5 21.5 16 — Horizontal
In order to define amethod to obtain directly fromcasting the cooling circuits a 125mm radius and 300mm length cylinder cavity to be produced into a chemically bounded sand mould was designed with placements for tubes. In this sandmould tubeswith different diameters andmaterials were tested, with and without internal sand as protective material for the tubes, and also a continuous gas flow was introduced to cool the tube during casting solidification. Definitively, standard AISI 316 stainless steel tubes were chosen for the internal cooling circuits, due to the low mismatch in composition between base alloy and AISI 316. On the other hand, zirconia sandwas selected as inside filler for the cooling tubes due to its high refractoriness.
We can observe in Table 2 the different tubes, fillers, and placement in respect to the parting line of the sand mould employed for casting trials as we can observe in Figure 2.
After pouring and subsequent solidification of the liquid composite material, casting part was cut and inspected to determinate if the tubes resisted the molten metal.
Optical microscopy has been used to determinate the structure of different alloys after heat treatments and also to determinate the coherency between the alloy and the tube material, in order to understand the obtained properties.
In order to test the materials in real production, a design and a cooling optimisation of real parts were made (see Figure 3(a)) and the patterns for sand mould were prepared, having in mind the support system for cores, as we can observe in Figure 3(b).
Internal tubes were cold deformed to obtain the desired forms and also in few cases arc welding technique was employed to obtain complex shapes.
In order to determinate a robust process, different cooling tubes in size and position and with and without internal insulating material (zirconia) defined in Table 2 were tested by using an induction furnace to cast steel over sand moulds with test tubes places into the mould cavity.
We can observe in Figure 4 how the tubes of Table 2 were placed in the sand test mould.
H13 base alloywas poured at 1560∘C (see Figure 5(a)), and after solidification, the test cylinder was cut (Figure 5(b)).
We can observe in Figure 5(a) how the metal solidifies into the sand die and in Figure 5(b) how only tubes filled with
International Journal of